#------------------------------------------------------------------------------
#$Date: 2024-08-03 13:19:43 +0300 (Sat, 03 Aug 2024) $
#$Revision: 293658 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/46/9004618.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9004618
loop_
_publ_author_name
'Cahill, C. L.'
'Krivovichev, S. V.'
'Burns, P. C.'
'Bekenova, G. K.'
'Shabanova, T. A.'
_publ_section_title
;The crystal structure of mitryaevaite,
 Al5(PO4)2[(P,S)O3(OH,O)]2F2(OH)2(H2O)8*6.48H2O, determined from a
 microcrystal using synchrotron radiation
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              179
_journal_page_last               186
_journal_paper_doi               10.2113/gscanmin.39.1.179
_journal_volume                  39
_journal_year                    2001
_chemical_formula_sum            'Al5 F2 H40 O32.48 P4'
_chemical_name_mineral           Mitryaevaite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                77.036
_cell_angle_beta                 73.989
_cell_angle_gamma                76.272
_cell_formula_units_Z            1
_cell_length_a                   6.918
_cell_length_b                   10.127
_cell_length_c                   10.296
_cell_volume                     663.714
_database_code_amcsd             0005711
_exptl_crystal_density_diffrn    2.144
_cod_original_formula_sum        'Al5 P4 O32.48 F2 H40'
_cod_database_code               9004618
loop_
_space_group_symop_operation_xyz
x,y,z
-x,-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
_atom_site_type_symbol
_atom_site_attached_hydrogens
Al1 0.02180 0.38400 0.21420 1.00000 ? Al 0
Al2 0.00000 0.00000 0.00000 1.00000 ? Al 0
Al3 0.49820 0.80200 -0.07380 1.00000 ? Al 0
P1 0.12430 0.05730 0.25640 1.00000 ? P 0
P2 0.10690 0.67040 0.04000 1.00000 ? P 0
O1 -0.00340 0.19990 0.27990 1.00000 ? O 0
O2 0.34540 0.06640 0.17840 1.00000 ? O 0
O3 0.02580 -0.01500 0.18170 1.00000 ? O 0
O-H4 0.13160 -0.03370 0.39880 1.00000 ? O 1
O5 -0.12340 0.39400 0.08440 1.00000 ? O 0
O6 0.02380 0.57490 0.17230 1.00000 ? O 0
O7 -0.03470 0.81310 0.03910 1.00000 ? O 0
O8 0.32500 0.68430 0.03870 1.00000 ? O 0
O-H9 0.27930 0.34200 0.09480 1.00000 ? O 1
F 0.27800 0.94660 -0.05730 1.00000 ? F 0
Wat10 0.55520 0.82350 0.09320 1.00000 ? O 2
Wat11 -0.23580 0.43120 0.34620 1.00000 ? O 2
Wat12 0.16150 0.37540 0.36040 1.00000 ? O 2
Wat13 0.42660 0.78550 -0.23990 1.00000 ? O 2
Wat14 0.14490 0.25320 0.62580 1.00000 ? O 2
Wat15 -0.59170 0.56450 0.29070 1.00000 ? O 2
Wat16 0.42100 -0.25210 0.44780 1.00000 ? O 2
Wat17 0.50000 0.00000 0.50000 0.48000 ? O 2
H1 -0.59200 0.63400 0.32100 1.00000 0.00170 H 0
H2 0.48200 0.89300 0.13500 1.00000 0.00350 H 0
H3 0.14200 0.31900 0.68500 1.00000 0.00210 H 0
loop_
_cod_changelog_entry_id
_cod_changelog_entry_author
_cod_changelog_entry_date
_cod_changelog_entry_text
1
;cod-tools version 3.8.0
Id: cif_guess_AMCSD_atom_types 9581 2023-05-17 12:35:41Z saulius
;
2023-05-18T11:38:21+03:00
;Derived atom types and hydrogen counts
from atom names that follow the AMCSD naming convention
(Wat == water, O-H == hydroxyl).
;
2
;cod-tools version 3.10.1
Id: cif_fix_AMCSD_aniso_labels 10200 2024-08-01 14:09:44Z saulius
;
2024-08-02T12:20:39+03:00
;Changed the following '_atom_site_aniso_label' values:
'OH4' -> 'O-H4'
'OH9' -> 'O-H9'
;
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0005711
